Delft University of Technology
Tests for the characterization of original Groningen masonry (C31B60-3)
Jafari, S.; Panoutsopoulou, L.; Rots, J.G.
Publication date
2015
Document Version
Final published version
Citation (APA)
Jafari, S., Panoutsopoulou, L., & Rots, J. G. (2015). Tests for the characterization of original Groningen
masonry (C31B60-3). Delft University of Technology.
Important note
To cite this publication, please use the final published version (if applicable).
Please check the document version above.
Copyright
Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy
Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.
This work is downloaded from Delft University of Technology.
Project number C31B60
File reference C31B60-3
Date 18 December 2015
Corresponding author Samira Jafari ([email protected])
Physical Testing and Modelling – Masonry Structures
TESTS FOR THE CHARACTERIZATION OF
ORIGINAL GRONINGEN MASONRY
Authors: Samira Jafari, Lydia Panoutsopoulou, Jan G. Rots
Collaborators: George Tzimiris, Zainab Aldin
Cite as: Jafari, S., Panoutsopoulou, L., Rots, J.G. Tests for the characterization of original Groningen masonry.
Report No. C31B60-3, 18 December 2015. Delft University of Technology.
This document is made available via the website ‘Structural Response to Earthquakes’ and the TU Delft repository. While citing, please verify if there are recent updates of this research in the form of scientific papers.
All rights reserved. No part of this publication may be reproduced, stored in a retrieval system of any nature, or transmitted, in any form or by any means, electronic, mechanical, photocopying, recording or otherwise, without the prior written permission of TU Delft.
TU Delft and those who have contributed to this publication did exercise the greatest care in putting together this publication. This report will be available as-is, and TU Delft makes no representations of warranties of any kind concerning this Report. This includes, without limitation, fitness for a particular purpose, non-infringement, absence of latent or other defects, accuracy, or the presence or absence of errors, whether or not discoverable. Except to the extent required by applicable law, in no event will TU Delft be liable for on any legal theory for any special, incidental consequential, punitive or exemplary damages arising out of the use of this report.
Material properties of original Groningen masonry ii
Table of Contents
1 Introduction ... 1
2 Nomenclature ... 2
3 Arrived samples ... 4
4 Compressive strength of masonry units ... 5
4.1 Testing procedure ... 5
4.2 Experimental results ... 6
5 Flexural strength of masonry units ... 10
5.1 Testing procedure ... 10
5.2 Experimental results ... 11
6 Compressive strength of masonry parallel to bed joints ... 18
6.1 Testing procedure ... 18
6.2 Experimental results ... 19
7 Bending strength of masonry ... 30
7.1 Testing procedure ... 30
7.2 Experimental results ... 31
8 Bond strength of masonry ... 38
8.1 Testing procedure ... 38
8.2 Elaboration of data ... 38
9 Compressive strength of masonry perpendicular to bed joints... 44
10 Shear strength of masonry ... 48
11 Summary-overview of material properties ... 50
References ... 51
Appendix A – Single Brick Compression ... 52
Appendix B – Single Brick Bending ... 53
Material properties of original Groningen masonry 1
1 Introduction
The NAM Hazard & Risk work as well as the NAM Structural Upgrading heavily depend on nonlinear finite element (FEM) analysis for masonry. In addition to nonlinear static push-over analyses, nonlinear dynamic time domain analyses become increasingly popular in order to assess the seismic capacity of Groningen buildings, of which 75% consist of masonry, see e.g. the Winningsplan research and the terraced house task force. These high-end analyses give direct engineering answers, but also serve as validation to simplified approaches that can then be inserted in large-scale probabilistic fragility studies or structural design. Nonlinear FEM codes employ constitutive models that describe the material behaviour. The constitutive models require input material parameters for stiffness, strength and ductility in compression, tension and shear. Subsets of those material parameters are also required for other purposes, like serving analytical structural models, and serving linear lateral force methods or linear response spectrum analyses where results in terms of generalized forces for masonry piers and spandrels have to be judged against material capacities. Apart from the obvious need for the validation of numerical models, it is furthermore necessary to calibrate in situ non-destructive test methods as a quick, cost effective (compared to more invasive techniques) and efficient way to determine the mechanical properties of masonry structures in the Groningen area.
In order to achieve both goals, an extensive testing program of the various types of in situ masonry was carried out, to investigate the mechanical properties of the original masonry and its constituent materials. In this document, the material properties of the original masonry are reported, as determined by tests carried out at the Stevin II Laboratory at TU Delft and TU/e laboratory. Samples have been tested both from residential buildings, as well as schools, dating from the 1920s up to 2013. The predominant masonry units used are clay bricks (mainly solid, but also perforated and frogged), there are several samples consisting of calcium silicate bricks, concrete blocks (both normal and aerated) or calcium silicate elements. To investigate the effects caused by the year of construction on the material properties, clay brick specimens are categorised into before and after 1945, and calcium silicate specimens are classified as before and after 1985.
2 Nomenclature
The symbols used in this report had been previously agreed upon among the partners of the testing program, and are not necessarily the same as in European codes and standards.
b
Mean width of bed joint1
d
Distance between bearing supports2
d
Distance between loading supports3
d
Distance between the loading and bearing supports in a four-point bending test bf
Masonry uniaxial bond strength between brick and mortar ,m h
f
Compressive strength of masonry in the direction parallel to the bed jointsv m
f
, Compressive strength of masonry in the direction perpendicular to the bed joints ,mu c
f
Compressive strength of masonry unitc bu
f
_{,} Normalised compressive strength of masonry unitt mu
f
_{,} Tensile strength of masonry unit derived by a three-point bending test2
x
f
Masonry bending strength with the moment vector orthogonal to the bed joints and in the plane of the wall (out-of-plane bending, crack plane perpendicular to bed joints)3
x
f
Masonry bending strength with the moment vector orthogonal to plane of the wall (in-plane _{bending) } ul
Length of the masonry unitu
h
Height of the masonry units
t
Thickness of the masonry specimen as built ut
Thickness of the masonry unitel
v
Vertical displacement corresponding to the load Fel1,
m h
E
Young’s modulus of masonry subject to a compressive loading parallel to the bed joints, _{evaluated at a stress equal to 0.3}_{f}m
2,
m h
E
Young’s modulus of masonry subject to a compressive loading parallel to the bed joints, _{evaluated at a stress equal to 0.7}_{f}m
h chord
E
_{,} Chord modulus of masonry subject to a compressive loading parallel to the bed joints, evaluated between 0.3fm and 0.7fmv chord
E
_{,} Chord modulus of masonry subject to a compressive loading perpendicular to the bed joints, evaluated between 0.3fm and 0.7fmc mu
E
_{,} Chord modulus of masonry unit calculated from compression test, evaluated between 0.3fm and 0.7fm) ( , ht mu
E
Chord modulus of masonry unit calculated from bending test from horizontal LVDT, evaluated between 0.3fm and 0.7fm) ( , vt mu
E
Chord modulus of masonry unit calculated from bending test from vertical LVDT, evaluated between 0.3fm and 0.7fm ) ( 2 ,fx h mE
Chord modulus of masonry calculated from out-of-plane bending test from horizontal LVDTs, evaluated between 0.3fm and 0.7fm) ( 2 ,fx v m
E
Chord modulus of masonry calculated from out-of-plane bending test from vertical LVDTs, evaluated between 0.3fm and 0.7fm) ( 3 ,fx h m
E
Chord modulus of masonry calculated from in-plane bending test from horizontal LVDTs, evaluated between 0.3fm and 0.7fm) ( 3 ,fx v m
E
Chord modulus of masonry calculated from in-plane bending test from vertical LVDTs, evaluated between 0.3fm and 0.7fm1
F
Applied vertical load (bond-wrench test)2
3
F
Vertical load due to the upper brick (bond-wrench test) elF
Selected vertical load value in the linear elastic stagemax
F
Maximum vertical loadbj b
f
_{,} Bond strength of masonryh c f
G
_{} _{,} Fracture energy in compression test (loading parallel to bed joints) vc f
G
_{,} Fracture energy in compression test (loading perpendicular to bed joints)W
Section modulus
Masonry (bed joint) shear strength coefficient 0v
3 Arrived samples
In total 318 samples arrived in the Stevin II laboratory at the Delft University of Technology from 19 different sources in the period of 26 of May till 10 of July; including 12 clay bricks specimens, 4 calcium silicate specimens, concrete block, aerated concrete and calcium silicate element specimens. Each source had its specific code. Figure 1 presents an overview of arrived samples.
Several samples arrived in such degree of disintegration that it was not possible to test them.
Figure 1 – Overview of arrived samples.
Table 1 provides a list of the samples, categorised by building code, which were available for each type of testing, as well as the disintegrated samples.
Table 1 – Overview of arrived samples.
Compression In-plane Out-of-plane Brick Compression Bending
BEA-S1 0 3 3 12 0 0 BEA-S2 0 3 3 12 0 0 HOO-H2 0 3 3 12 0 3 KWE-H1 0 3 1 12 0 0 MID-H1 0 0 0 12 0 0 MOL-H1 0 0 0 12 0 0 ROE-S1.1 0 3 0 12 0 0 ROE-S1.2 0 3 0 12 0 0 ROE-S2 0 3 3 12 0 0 ROE-S3 0 3 3 12 0 1 WIL-H2 7 3 3 12 1 0 WIR-H1 3 3 3 12 1 0 BEA-H1 3 3 3 12 1 4 LAG-H2 3 3 3 12 0 4 SCH-H1 0 3 3 12 0 3 WIL-H1 3 3 6 12 0 6
Concrete Block JUL-H1 0 3 0 12 0 0
Aerated Concrete HOO-H1 3 3 2 0 0 0
CS Element JOH-H1 0 3 2 0 0 0 Number of disintegrated specimens Clay CS
4 Compressive strength of masonry units
Compression tests on masonry units were performed in accordance with EN 772-1:2011. The test allows the determination of the compressive strength of the units. In order to find Young’s modulus, vertical LVDTs were attached to measure relative displacement between upper and lower platens.
4.1 Testing procedure
For each code six masonry units were tested by having the bed joint plane perpendicular to the loading direction (Figure 2). Table 2 and Table 3 list the average dimensions of the masonry units tested.
The test was carried out by a load-controlled apparatus including a hydraulic jack with 350-ton capacity. The hydraulic jack lifts a steel plate, the active side, and there is a passive load plate at the top. A hinge between the load cell and the top steel plate reduces possible eccentricities during loading. A load cell that measures the applied force is attached to the top steel plate. The rate of loading was set so that maximum load was reached within 2 min, according to the standard.
Since the small height of the bricks did not allow attaching LVDTs in this dimension, four vertically oriented LVDTs were attached to measure relative vertical displacements between machine platens. The LVDTs have a measuring range of 10 mm with an accuracy of 0.5%.
Figure 2 – Compression test on brick.
In order to achieve more accurate values of Young’s modulus, it is anticipated to carry out compression tests on a pile of five bricks, bonded together with a very thin layer of special plaster. This set up was proposed in previous research and reported in CUR report 171 (1994).
Table 2 – Average dimensions of the clay masonry units. Masonry type Sample _{name } lu tu hu Type
mm mm mm Clay bricks BEA-S1 205 99 51 Solid KWE-H1 210 99 50 Solid HOO-H2 209 98 61 Frogged MOL-H1 212 103 51 Solid ROE-S1.1 210 102 62 Solid ROE-S3 205 95 49 Solid WIR-H1 219 110 53 Solid
Masonry type Sample _{name } lu tu hu Type mm mm mm Calcium silicate bricks BEA-H1 212 104 52 Solid LAG-H2 214 100 67 Solid SCH-H1 217 100 72 Solid WIL-H1 214 102 52 Solid
4.2 Experimental results
Assuming a linear stress distribution over the loaded cross section of the brick, the compressive strength,
fmu,c ,the normalised compressive strength, fbu,c and the elastic modulus, Emu,c of the brick can be determined
from the compression test as follows:
(1) (2) (3)
Where Fmax is the maximum load, A is the cross section of brick; Fel and εave are the load and the average of
strain of vertical LVDTs in the linear elastic stage, respectively.
Afterwards, the obtained values of the compressive strength were normalised according to Annex A of EN 772-1, by multiplication with the appropriate shape factor, d, for each case.
Table 4 and Table 5 present the values of compressive strength and chord modulus1_{ in the linear stages for }
clay and calcium silicate bricks as well as the normalised compressive strength of units. As mentioned before new tests are anticipated for investigation of more accurate values of Young’s modulus for units.
Figure 3 shows the histograms of normalised compressive strength for clay and calcium silicate masonry categorised according to the year of construction.
Appendix A shows the typical stress-strain diagrams in which the strain is an average of LVDTs readings and present the force-jack displacement curves for the six bricks from BEA-S1, LAG-H2 and HOO-H2.
Table 4 – Compressive strength and chord modulus for clay bricks.
1_{The slope of the chord drawn between 30% and 70% of the maximum stress on the stress-strain curve.}
A
F
f
muc max ,
c mu c bud
f
f
,
, ave el c muA
F
E
,Clay bricks < 1945 Clay bricks > 1945 Sample name Year of Cons
fmu.c Emu.c Shape
factor fbu.c _{Sample } name Year of Cons
fmu.c Emu.c Shape
factor fbu.c
MPa GPa MPa MPa GPa MPa
WIR-H1 1920 27.46 1.13 0.76 20.81 BEA-S1 1955 48.10 3.12 0.75 36.17 33.61 3.19 0.77 25.88 18.99 0.69 0.76 14.49 35.64 5.57 0.75 26.77 24.46 1.06 0.76 18.71 35.42 4.02 0.76 26.37 30.21 1.44 0.78 23.47 21.28 1.88 0.76 16.24 24.80 0.64 0.75 18.60 55.21 - 0.75 41.19 39.71 1.80 0.76 30.02 ROE-S1.1 1922 24.05 0.46 0.77 18.45 ROE-S3 1985 30.68 1.67 0.74 22.70 19.97 0.32 0.79 15.72 36.34 0.91 0.74 27.00 24.13 0.43 0.78 18.72 33.69 0.88 0.74 24.93 23.64 0.32 0.76 18.04 34.04 0.60 0.75 25.60 21.16 0.24 0.82 17.31 29.05 0.88 0.74 21.64 19.58 0.48 0.83 16.23 29.07 0.76 0.75 21.71 MOL-H1 1932 31.18 1.19 0.75 23.35 KWE-H1 1995 19.59 0.24 0.75 14.59 27.90 0.97 0.74 20.62 19.32 0.14 0.75 14.41 23.40 0.86 0.75 17.64 23.70 0.18 0.75 17.80 32.71 0.95 0.76 24.70 24.25 - 0.75 17.85 29.79 - 0.75 22.34 18.67 0.34 0.77 14.30 17.77 0.29 0.75 13.24 HOO-H2 2013 9.41 0.44 0.82 7.75 10.46 0.56 0.82 8.56 12.90 1.52 0.82 10.64 10.05 0.52 0.82 8.25 11.04 0.83 0.85 9.36 21.99 0.95 0.82 18.10 Weighted
average 28.62 1.51 0.77 21.78 Weighted average 24.10 0.86 0.77 18.33 Standard
deviation 8.71 1.58 0.02 6.24 deviation Standard 10.06 0.67 0.03 7.31 Coefficient of
variation 0.30 1.04 0.03 0.29 Coefficient of variation 0.42 0.78 0.04 0.40
Table 5 – Compressive strength and chord modulus for calcium silicate bricks <1985. Calcium silicate bricks < 1985
Sample name
Year of Cons
fmu.c Emu.c Shape
factor fbu.c
MPa GPa MPa
WIL-H1 1952 8.81 0.74 0.75 6.59 11.36 0.64 0.76 8.64 7.33 0.38 0.77 5.64 20.85 0.80 0.78 16.24 BEA-H1 1958 31.37 5.14 0.75 23.37 22.45 2.80 0.75 16.72 24.16 3.10 0.75 18.00 20.35 2.05 0.75 15.16 21.68 3.07 0.75 16.15 20.49 3.03 0.76 15.26 LAG-H2 1978 13.83 3.76 0.87 12.03 17.47 2.24 0.86 15.07 18.88 2.31 0.87 16.44 20.32 3.72 0.87 17.68 22.25 4.69 0.88 19.49 20.76 5.24 0.88 18.18 SCH-H1 1978 18.19 3.04 0.87 15.86 17.19 4.49 0.87 14.90 15.49 1.64 0.87 13.51 22.33 3.27 0.87 19.36 19.21 3.29 0.87 16.66 19.85 3.36 0.87 17.21 Weighted average 18.28 2.67 0.81 14.86 Standard deviation 5.24 1.41 0.06 4.13 Coefficient of variation 0.29 0.53 0.07 0.28
(a) (b)
5 Flexural strength of masonry units
Three-point bending tests on masonry units were performed in agreement with NEN 6790:2005. The test allows determining the flexural tensile strength and the elastic modulus of the masonry unit.
5.1 Testing procedure
The masonry units (Figure 4) were tested by having the bed joint plane parallel to the loading direction. The specimen was supported by two roller bearings, which were placed 10 mm from the end of specimen. A third roller was used to apply load to the specimen at mid-span. Table 6 and Table 7 list the average dimensions of the masonry units and the distance between the supports.
The test is carried out by a displacement-controlled apparatus including a hydraulic jack with 10-ton capacity. To obtain the failure of the specimen in 30 to 90 s, a displacement rate of 0.03 mm/s is adopted. The applied load is recorded from the load cell attached to the hydraulic jack.
Two LVDTs are attached to the specimens to measure horizontal and vertical displacements. On the front side, a horizontal LVDT measures the elongation between two points on the masonry unit (Figure 5a). On the back side the vertical displacement is measured at mid-span of the masonry unit, relative to its supports (Figure 5b). The LVDTs have a measuring range of 10 mm with an accuracy of 0.5%.
(a) (b)
Figure 4 – (a) Clay brick; (b) Calcium silicate brick.
Table 6 –Average dimensions of the clay units and distance between the bearing supports. Masonry type Sample _{name } lu tu hu d1 Type
mm mm mm mm Clay bricks BEA-S1 207 99 61 197 Solid BEA-S2 211 100 59 201 Perforated KWE-H1 215 106 61 205 Solid HOO-H2 212 100 61 202 Frogged MID-H1 210 100 52 200 Solid MOL-H1 212 103 51 202 Solid ROE-S1.1 210 102 62 200 Solid ROE-S1.2 206 97 59 196 Solid ROE-S2 215 107 51 205 Solid ROE-S3 205 95 49 195 Solid WIL-H2 231 102 65 221 Solid WIR-H1 219 110 53 198 Solid
Table 7 – Average dimensions of the calcium silicate bricks and concrete block units and distance between the bearing supports.
Masonry type Sample _{name } lu tu hu d1 Type mm mm mm mm Calcium silicate bricks BEA-H1 212 104 52 192 Solid LAG-H2 214 100 67 204 Solid SCH-H1 217 100 72 207 Solid WIL-H1 214 102 52 193 Solid
Concrete block JUL-H1 214 102 93 204 Perforated-Solid
(a) (b)
Figure 5 – Three-point bending flexural test on bricks (a) horizontal LVDT (b) vertical LVDT.
5.2 Experimental results
Assuming a linear stress distribution over the height of the brick’s cross-section, the tensile strength, fmu,t and
the elastic modulus, Emu,t of the masonry units can be determined from the vertical and horizontal LVDTs from
the three-point bending test as follows:
(4)
(5) (6)
Where Fmax is the maximum load, d1 is the distance between the supports, hu is the height of the masonry
unit, tu is the thickness of the masonry unit, Fel and vel are the load and vertical displacement in the linear
elastic stage, respectively. I is the moment of inertia of the masonry unit along the cross-section and ƙ is curvature (The strain from the horizontal LVDT divided by the distance of the LVDT from the neutral axis). In the case of perforated bricks, the reduced moment of inertia is considered.
If the masonry unit fails at the support, a shear failure is obtained rather than bending failure. As a consequence, the elastic modulus cannot be calculated. Table 8 to Table 14 list the results in terms of flexural tensile strength and in terms of the elastic modulus from vertical and horizontal LVDTs.
The weighted average2_{ value of flexural strength for solid clay bricks before and after 1945 is 6.43 and 4.69 }
MPa, respectively. Most of the bricks from the individual sample codes are almost in this range except bricks
2_{ An average in which each sample is assigned a weight according to the number of available samples from }
each code. max 1 , 2
3
2
mu t u uF
d
f
h t
I
v
d
F
E
el el v t mu48
3 1 ) ( ,
I
M
E
_{mu}_{,}_{t}_{(}_{h}_{)}
belonging to MID-H1, which showed high values of flexural strength, averaging 10.42 MPa. The calcium silicate bricks present the weighted average flexural strength of 4.44 MPa.
As for the Young’s modulus, the weighted average value for solid clay bricks before and after 1945 determined from the vertical displacement measurements are 12.8 and 8.4 GPa respectively, whereas from the horizontal ones are equal to 29.4 and 18.6 GPa, respectively. For the calcium silicate samples, the obtained values from vertical and horizontal LVDTs are 10.7 GPa and 23.8 GPa respectively. In all cases, the Young’s modulus from vertical measurements is two to three times lower than from the horizontal measurements.
Figure 6 shows the crack pattern for different types of the bricks including calcium silicate, perforated clay brick and concrete block.
Appendix B shows the typical flexural stress-displacement diagrams for each code of bricks. The bricks present a brittle failure when the maximum force is reached.
Figure 7 shows the histograms of flexural strength for solid clay bricks and calcium silicate bricks.
(a) (b) (c)
Figure 6 – Crack pattern: (a) calcium silicate brick; (b) symmetric crack pattern for clay brick; (c) crack pattern for concrete block.
(a) (b)
Figure 7 – Histograms of flexural strength: (a) solid - clay bricks; (b) calcium silicate bricks. Table 8 – Flexural strength and elastic modulus for solid-clay-brick bricks < 1945.
Solid-clay-brick <1945
Year of
Cons Average Average Average
MID-H1 1920 10.85 10.42 55.9 45.03 20.3 14.88 8.18 44.9 - 8.23 35.3 13.3 8.86 36.9 20.4 17.35 45.4 6.0 9.05 51.8 14.4 WIR-H1 1920 7.63 4.73 25.7 28.22 - 9.89 6.22 22.6 12.4 2.71 - 9.1 6.04 35.4 - 3.74 30.3 9.2 3.57 - 5.9 6.36 - 13.4 3.24 29.2 9.7 1.77 14.9 7.4 3.41 21.4 7.0 9.38 64.1 20.0 2.68 10.4 4.8 ROE-S1.1 1922 1.54 4.51 4.7 19.85 1.6 7.63 6.22 28.3 1.6 1.02 1.7 1.1 6.33 27.8 11.3 9.79 43.9 25.8 2.17 12.7 4.4 ROE-S1.2 1922 12.21 9.73 64.5 42.38 26.6 24.72 8.39 37.0 29.2 7.58 25.7 20.9 2.87 21.1 10.5 13.79 60.5 31.9 13.51 45.5 29.2 MOL-H1 1932 3.42 2.78 15.0 11.57 10.7 8.69 1.69 11.3 3.9 6.60 23.8 15.2 2.76 7.3 - 0.71 0.9 0.5 1.49 11.1 13.15 Weighted average 6.43 29.41 12.76 Standard deviation 4.11 18.03 8.91 Coefficient of variation 0.53 0.61 0.70
Table 9 – Flexural strength and elastic modulus for solid clay bricks > 1945. Solid-clay-brick > 1945
Sample name Year of _{Cons } fmu.t [MPa] Emu.t(h) [GPa] Emu.t(v) [GPa]
Average Average Average
BEA-S1 D1 1955 3.17 4.06 20.3 18.58 12.3 9.96 D2 4.98 25.0 11.7 D3 4.70 21.8 13.1 D4 4.76 14.6 9.5 D5 2.67 11.2 3.2 KWE-H1 D1 1995 4.11 5.22 15.3 17.80 10.6 7.18 D2 4.50 19.3 3.6 D3 5.80 20.9 7.5 D4 4.98 20.6 - D5 6.19 - 10.9 D6 5.71 12.9 3.3 ROE-S2 D1 1955 1.98 2.80 3.3 11.07 1.3 4.65 D2 2.41 9.3 1.6 D3 2.63 12.4 4.8 D4 4.46 22.3 9.3 D5 3.58 13.5 5.9 D6 1.75 5.6 5.0 ROE-S3 D1 1985 8.74 6.46 24.7 20.34 13.4 11.86 D2 8.79 19.8 11.2 D3 5.31 25.1 11.1 D4 3.27 9.9 8.8 D5 6.17 22.2 14.8 WIL-H2 D1 1952 7.68 4.94 30.5 25.37 - 8.17 D2 2.71 15.3 3.8 D3 4.96 35.4 10.9 D4 6.60 25.2 - D5 2.60 22.4 - D6 5.09 23.4 9.8 Weighted average 4.69 18.63 8.36 Standard deviation 1.90 7.42 4.04 Coefficient of variation 0.40 0.40 0.48
Table 10 – Flexural strength and elastic modulus for perforated clay bricks. Perforated -clay-brick > 1945
Sample name Year of _{Cons } fmu.t [MPa] Emu.t(h) [GPa] Emu.t(v) [GPa]
Average Average Average
BEA-S2 D1 2001 4.2 3.38 13.5 12.75 11.7 8.23 D2 3.4 12.6 9.9 D3 3.0 11.6 5.6 D4 3.2 13.0 8.7 D5 3.0 12.5 3.6 D6 3.5 13.3 9.9 Weighted average 3.38 12.75 8.23 Standard deviation 0.45 0.68 3.04 Coefficient of variation 0.13 0.05 0.37
Table 11 – Flexural strength and elastic modulus for frogged clay bricks. Frogged-clay brick > 1945
Sample name Year of _{Cons } fmu.t [MPa] Emu.t(h) [GPa] Emu.t(v) [GPa]
Average Average Average
HOO-H2 D1 2013 2.8 3.18 18.4 14.58 12.4 8.20 D2 4.3 15.6 7,7 D3 1.3 10,2 6.8 D4 3.3 7.6 8.1 D5 2.5 15.4 6.5 D6 4.9 20.3 7.7 Weighted average 3.18 14.58 8.20 Standard deviation 1.29 4.84 2.14 Coefficient of variation 0.41 0.33 0.26
Table 12 – Flexural strength and elastic modulus for concrete block. Concrete block
Sample name Year of _{Cons } fmu.t [MPa] Emu.t(h) [GPa] Emu.t(v) [GPa]
Average Average Average
JUL-H1 D1 1957 1.7 1.27 14.5 12.6 10.6 7.3 D2 1.5 15.3 - D3 2.4 17.9 10.4 D4 0.4 10.2 9.2 D5 1.2 - 5.4 D6 0.4 5.2 1.0 Weighted average 1.27 12.6 7.3 Standard deviation 0.78 5.0 4.1 Coefficient of variation 0.61 0.40 0.56
Table 13 – Flexural strength and elastic modulus for calcium silicate bricks < 1985. Calcium Silicate bricks
Sample name Year of Cons
fmu.t [MPa] Emu.t(h) [GPa] Emu.t(v) [GPa]
Average Average Average
BEA-H1 D1 1958 6.07 4.05 35.0 23.4 - 10.3 D2 4.02 18.8 - D3 2.14 21.6 2.4 D4 3.25 18.4 1.1 D5 3.18 28.3 11.2 D6 4.32 0.6 0.8 D7 3.32 27.7 23.9 D8 3.04 27.5 - D9 3.55 27.2 - D10 6.25 - 24.6 D11 2.84 17.5 8.0 D12 6.66 34.3 - LAG-H2 D1 1978 5.43 4.52 30.3 27.2 14.2 10.2 D2 3.41 25.9 8.4 D3 4.66 26.2 8.5 D4 5.25 27.5 10.1 D5 4.02 18.9 9.4 D6 3.88 23.3 9.2 D7 4.28 24.5 8.7 D8 4.69 30.4 12.6 D9 4.50 32.1 10.1 D10 5.31 33.4 12.1 D11 4.20 30.9 7.5 D12 4.55 22.8 11.5 SCH-H1 D1 1978 5.55 5.01 29.2 27.7 15.1 13.1 D2 4.55 29.6 - D3 5.59 28.4 - D4 4.99 24.9 - D5 3.78 23.7 9.5 D6 5.57 30.1 14.8 WIL-H1 D1 1952 2.70 4.2 11.7 18.1 - 8.8 D2 2.58 12.5 2.6 D3 1.95 15.5 3.9 D4 2.17 1.5 - D5 7.97 12.8 15.2 D6 4.47 31.0 8.4 D7 4.98 26.7 17.7 D8 3.44 16.0 11.3 D9 8.36 35.7 - D10 7.37 - -
Table 14 – Flexural strength and elastic modulus for calcium silicate bricks < 1985. Calcium Silicate bricks
Sample name fmu.t [MPa] Emu.t(h) [GPa] Emu.t(v) [GPa]
Average Average Average
WIL-H1 D11 1.16 4.2 - 18.1 2.2 8.8
D12 3.11 17.3 -
Weighted average 4.44 23.8 10.7
Standard deviation 1.58 8.6 5.7
6 Compressive strength of masonry parallel to bed joints
The compression strength and Young’s modulus of the masonry when the load is parallel to the bed joints are determined in agreement with EN 1052-1:1998. Some variations are adopted to investigate the orthotropic behaviour of the masonry and the cyclic response of the material.
6.1 Testing procedure
The compression strength and Young’s modulus of the masonry are determined along the direction when the load is parallel to the bed joints3_{. Figure 8 shows the adopted configuration. }
The sizes of the arrived samples were in agreement with EN 1052-1:1998. The three clay masonry wallettes from WIL-H2(F1/2/4) had two bricks in height and eight rows of bricks in length (2x8x1-brick) and specimens from WIR-H1 and WIL-H2-(C1/2/3) had two bricks in height and seven rows of bricks in length (2x7x1-brick). The calcium silicate masonry wallettes from BEA-H1 and WIL-H1 had dimensions of (2x7x1-brick) and specimens from LAG-H2 had two full bricks in height and five rows of bricks in length. A 10 mm thick layer of gypsum is applied to bring the faces in contact with the loading plates, to ensure that the loaded faces of the specimens are levelled and parallel to one another.
The testing apparatus is provided with a 350 tons hydraulic jack, positioned at the bottom. The hydraulic jack lifts a steel plate, the active side, and there is a passive load plate at the top. A hinge between the load cell and the top steel plate reduces possible eccentricities during loading. The hydraulic jack is operated deformation controlled, using the jack displacement as control variable. A load cell that measures the applied force is attached to the top steel plate.
Four LVDTs (two for each side) are attached to the specimen in accordance with EN1052-1:1998 to register vertical relative displacements over the height of the specimen. They are installed as closely as possible to the surface of the specimen to reduce possible errors caused by rotation of the contact points to which they are attached. Their measuring range is 5 mm with an accuracy of 0.5%.
Two LVDTs (one for each side) are attached to the specimen to register the horizontal relative displacement over the length of the specimen. Their measuring range is 2 mm with an accuracy of 0.5%.
Three samples from BEA-H1, WIL-H1/2, LAG-H2 and WIR-H1 were tested by applying a monotonic loading as prescribed by EN 1052-1:1998. Half of the expected maximum compression force is applied in three equal steps and is kept constant for 2 min ± 1 min. Afterwards the maximum stress in reached monotonically. Subsequently the test is continued to explore the post-peak behaviour. The load is applied at a rate of 0.002 mm/s in order to reach the peak stress in 15 to 30 min. The deformation and the force are registered, including the post-peak softening regime.
For each of the codes WIL-H2 and HOO-H1 three samples were tested by applying a cyclic loading. This loading configuration is not prescribed by the standard, but it is in line with tests performed in TU/e. It gives additional information regarding the loading-unloading behaviour. The target is to have at least three cycles before the maximum force. As a result the loading and unloading is carried out with increments of 50 kN. The load is applied with a rate of 0.006 mm/s in order to reach the peak stress in approximatively 30 min. The deformation and the force are registered.
Figure 8 – Compression test on masonry: Horizontal configuration (loading direction parallel to bed joint).
(a) (b)
(c) (b)
Figure 9 – Position of the LVDTs during the compression test on masonry: (a) Clay masonry samples (b); (c) Calcium silicate masonry and (d) Aerated concrete wallettes.
6.2 Experimental results
Assuming the stress is constant over the cross-section of the specimen, the compressive strength of masonry for horizontal, fm,h, configuration can be determined as follows:
(7)
Where Fmax is the maximum load, hs and tsare the dimensions of the masonry specimens.
During the test the displacements and the force are measured continuously allowing the determination of the stress-strain relationship. Form this relation is it possible to determine the Young’s modulus of masonry. Three estimations of the Young’s modulus are adopted here:
Em1,h is the secant Young’s modulus evaluated at 30% of the ultimate strength;
Em2,h is the secant Young’s modulus evaluated at 70% of the ultimate strength;
load cell hinge top steel plate
bottom steel plate
jack LVDT masonry specimen max , m h s s
F
f
t h
hs hs hs hs Echord,h is the chord modulus evaluated in the elastic stage that in the most cases is calculated
between 30% and 70% of the ultimate strength.
The displacement control procedure of the test allows determining the post-peak behaviour of the material. The fracture energy Gf-c in compression can be determined as the area underneath the stress-displacement
diagram, while the displacement can be obtained from the LVDTs displacement or the jack displacement. It should be mentioned that calculating the fracture energy from the jack displacement, in most cases, leads to the overestimation, since the jack displacement also includes the gypsum deformation. Accordingly, the fracture energy is calculated, here, from the LVDTs displacement. In this study, it is assumed that the fracture energy, calculated from the LVDTs displacement is mapped back to the whole specimen height, but without the gypsum deformation, by multiplying it with the ratio of specimen height versus LVDT height. As a result, the fracture energy is calculated from the LVDTs outputs, as follows:
LVDT specimen LVDT LVDT h m c f
Height
Height
d
L
f
G
_{}
_{,}.
.
(8)Table 15 and Table 16 list the main experimental results for the clay masonry wallettes.
Figure 10 and Figure 11 show the stress-strain diagram for the clay masonry under horizontal compression. In the graphs, the terminology normal strain identifies the deformation in the direction of the loading, while the term lateral strain defines the deformation in the orthogonal direction. Both deformations are the average of the LVDTs readings. The pre-peak stage is characterized by linear-elastic behaviour up to 1/3 of the maximum stress followed by a parabolic non-linear behaviour. Due to the extensive cracking the LVDTs can detach; thus the post-peak behaviour can be retrieved by analysing the displacement of the jack (Figure 12). Figure 13 displays the development of cracks in samples tested under horizontal compression. Cracks start in the bricks and are oriented parallel to the loading direction (Figure 13a, Figure 13b). In the post peak phase, the external surface of the bricks is spalled (Figure 13c, Figure 13d).
Table 15 – Results of horizontal compressive tests on clay masonry wallettes < 1945. Sample name Test
type
Year of Cons
fm,h Mean Em1,h Em2,h Echord,h Mean Gf-c,h Mean
MPa MPa MPa MPa N/mm
WIR-H1 C1 monotonic 1920 11.73 10.86 13556 11695 10602 8933 30.84 30.84
C2 9.99 11341 8587 7264 -
Weighted average 10.86 12449 10141 8933 30.84
Standard deviation 1.23 1566 2198 2360 -
Table 16 – Results of horizontal compressive tests on clay masonry wallettes > 1945. Sample name Test _{type } Year of
Cons
fm,h Mean Em1,h Em2,h Echord,h Mean Gf-c,h Mean
MPa MPa MPa MPa N/mm
WIL-H2 F1 monotonic 1952 7.41 11.00 6697 5791 5183 5470 22.80 31.55 F2 8.97 6383 5340 4756 - F4 10.58 7486 6095 5349 - C4 cyclic 14.23 7979 6291 5428 - C5 12.57 8731 7175 6327 40.30 C6 12.22 9062 7017 5778 - Weighted average 11.00 7723 6285 5470 31.55 Standard deviation 2.51 1075 707 536 12.37 Coefficient of variation 0.23 0.14 0.11 0.10 0.39
Figure 11 – Horizontal compression tests on clay masonry wallettes.
Figure 12 – Stress-strain curve derived by LVDTs and jack readings for clay masonry wallettes.
(a) (b) (c) (d)
Figure 13 – Crack pattern of wallette tested under horizontal compression test: (a) First crack; (b) Maximum stress; (c)-(d) Post-peak phase.
Figure 14 and Figure 15 show the stress-strain diagram for the calcium silicate masonry under horizontal compression. In the graphs, the terminology normal strain identifies the deformation in the direction of the loading, while the term lateral strain defines the deformation in the orthogonal direction. Both deformations are the average of the LVDTs readings. The pre-peak stage is characterized by linear-elastic behaviour up to 1/3 of the maximum stress followed by a parabolic non-linear behaviour. Due to the extensive cracking the LVDTs can detach; thus the post-peak behaviour can be retrieved by analysing the displacement of the jack (Figure 16).
Figure 17 analyses the development of cracks in samples tested under horizontal compression. Horizontal cracks start in the mortar-brick interface for the head joints, at one of the outer surfaces, similar to buckling (Figure 17a). When the maximum stress is reached, vertical cracks develop in the bricks while the damage is concentrated in the bottom or upper part, where half bricks are located (Figure 17b). In the post peak phase, the vertical cracks appear both in the bricks and the bed joints, which are aligned with the loading direction (Figure 17c, Figure 17d).By analysing the crack pattern, it is interesting to note that in this case, the damage is mainly located in the brick-mortar interfaces. Bricks and head joints form small columns which are subject to buckling rather than cracking in the bricks.
Figure 18 to Figure 20 show the histograms of compressive strength, chord modulus and fracture energy for clay masonry and calcium silicate masonry wallettes.
Table 17 – Results of horizontal compressive tests on calcium silicate masonry wallettes < 1985. Sample
name Year of Cons type Test
fm,h Mean Em1,h Em2,h Echord,h Mean Gf-c,h Mean
MPa MPa MPa MPa N/mm
BEA-H1 C4 1958 monotonic 4.93 4.24 7620 3633 4788 5375 15.35 15.35 C5 3.55 4647 5317 5961 - LAG-H2 C4 1978 monotonic 7.52 7.53 4174 2995 2474 3386 26.89 18.86 C5 6.68 5640 3188 2405 15.16 C6 8.39 6682 5803 5280 14.54 WIL-H1 C4 1952 monotonic 6.75 7.01 5615 5034 4671 4450 21.23 20.80 C5 8.00 8453 6925 6103 - C6 6.27 2985 2736 2576 20.37 Weighted average 6.26 5772 4456 4404 18.34 Standard deviation 1.61 1814 1529 1569 2.76 Coefficient of variation 0.26 0.31 0.34 0.36 0.15
Figure 14 – Horizontal compression tests on calcium silicate masonry wallettes.
Figure 16 – Stress-strain curve derived by LVDTs and jack readings for calcium silicate masonry wallettes.
(a) (b) (c) (d)
Figure 17 – Crack pattern of CS wallette tested under horizontal compression test: (a) First crack; (b) Maximum stress; (c)-(d) Post-peak phase.
(a) (b)
(a) (b)
Figure 19 – Histograms of Young’s modulus: (a) clay masonry; (b) calcium silicate masonry.
(a) (b)
Figure 20 – Histograms of fracture energy: (a) clay masonry; (b) calcium silicate masonry.
Figure 21 shows the stress-strain diagram for the aerated concrete wallettes under horizontal cyclic compression. In the graphs, the terminology normal strain identifies the deformation in the direction of the loading, while the term lateral strain defines the deformation in the orthogonal direction. Both deformations are the average of the LVDTs readings. The pre-peak stage is characterized by linear-elastic behaviour up to 1/3 of the maximum stress followed by a parabolic non-linear behaviour.
Figure 22 analyses the development of cracks in samples tested under horizontal compression. Vertical cracks start in the surface of samples and are oriented parallel to the loading direction (Figure 22a, Figure 22b). In the post peak phase, deep cracks split the wallettes into different columns (Figure 22c, Figure 22d).
Table 18 lists the main experimental results for the aerated concrete wallettes.
Table 18 – Results of horizontal compressive tests on aerated concrete wallettes. Sample name Year of _{Cons } Test _{type } fm,h Em1,h Em2,h Echord,h Gf-c,h
MPa MPa MPa MPa N/mm
HOO-H1 C1 2013 cyclic 1.17 640 602 577 5.30
C3 2.96 1698 1167 946 5.57
Average 2.18 1164 968 881 6.96
Standard deviation 0.92 529 318 278 2.64
Figure 21 – Horizontal compression tests on aerated concrete wallettes.
(a) (b) (c) (d)
Figure 22 – Crack pattern wallette HOO-H1 tested under horizontal compressive test: (a) First crack; (b) Maximum stress; (c)-(d) Post-peak phase.
7 Bending strength of masonry
The bending strength of masonry is determined for two configurations:
Four-point bending with the moment vector orthogonal to the bed joints and in the plane of the wall (Bending test Out-of-Plane, with the crack plane orthogonal to the bed joints) and
Four-point bending with the moment vector orthogonal to plane of the wall (Bending test In-Plane with the crack plane orthogonal to the bed joints).
The first test is performed in agreement with EN 1052-2:1999, while the second one is a non-standardised test. The in-plane test is carried out in the same way as the out-of-plane test with the specimen rotated by 90 degrees as seen in Figure 23 b.
7.1 Testing procedure
Masonry samples were delivered for 17 different objects, 16 of which were tested. All the samples for WIL-H-1 had been broken on arrival; hence no tests could be performed for this particular object. For WIL-H-12 of the objects, the samples tested were 4x4 brick wallettes, with the distance between the supports, d1, equal to
720 mm and the distance between the points of load application, d2, equal to 360 mm. For the in-plane
testing, one sample from LAG-H-2 and two samples from JUL-H-1 were saw-cut to 4x3 brick, since the larger height of the comprising units did not allow for a purely flexural behaviour of the samples. For HOO-H-1 and JOH-H-1 the samples measured 600x200 mm, with d1 = 495 mm and d2 = 220 mm.
The masonry specimens were subjected to a four-point bending test (Figure 23). The load was transferred to the sample via steel profiles. To have an uniform distribution of the load along the thickness of the specimen, rubber strips were placed between the masonry specimen and the loading frame. The loading frame distributed linear loads over two supporting rollers. The distance between the loading rollers, d2, and bearing
rollers, d1, as chosen in agreement with the prescription of EN 1052-2:1999. A ratio of d2 / d1 = 0.5 was
chosen.
The load was applied in displacement control by a spherical joint attached to a hydraulic jack with 10 tons capacity. The displacement rate of the piston of the jack was 0.002 mm/s. The applied load was recorded from the load cell attached to the hydraulic jack.
For each side 5 LVDTs were attached to measure the vertical and horizontal displacements including four vertical LVDTs and one horizontal LVDT. However when there is not a head joint in the middle of the specimen, 3 vertical LVDTs were attached instead of 4, since the mid-span displacement could be obtained accurately using only one LVDT in that position. The LVDTs had a measuring range of 10 mm with an accuracy of 0.5%.
(a) (b)
7.2 Experimental results
These tests allowed determining the flexural strength fx as follows:
(9)
Where Mmax is the maximum bending moment, Fmax is the maximum load at failure, d3 is the distance between
the loading and the bearing supports, W is the section modulus.
The Young’s modulus of the specimens was calculated as the chord modulus between 30% and 70% of the flexural strength from vertical and horizontal LVDTs.
Appendix C shows the force – mid-span displacement and moment – curvature (The strain from the horizontal LVDT divided by the distance of the LVDT from the neutral axis) curves for the specimens subject to out-of-plane bending. The mid-span displacement has been either calculated from the readings of the vertical LVDTs through linear interpolation, or obtained directly from the measurements of a LVDT positioned there, whenever that was possible. In all cases, the behaviour of the samples was very brittle, with instantaneous failure at the formation of a single crack. Three main crack patterns were observed: a) A single, straight crack was formed at or close to one of the points of load application, b) a single, straight crack at mid-span, and c) a straight crack at mid-span with debonding of the middle brick in the last row. These patterns are shown in Figure 24 and Figure 25. In almost all cases, the observed crack propagated along the brick-mortar interface and through any bricks in its path. The obtained results are presented in Table 19 to Table 22 according to masonry unit type and years of construction.
Figure 26 shows the results as a histogram plot for all types of clay bricks masonry.
(a) (b)
Figure 24 – Out-of-Plane Bending – Typical crack patterns: (a) Straight crack at the point of load application; (b) Straight crack at the middle of the specimen.
Figure 25 – Out-of-Plane Bending – Typical crack patterns: Straight crack at the middle and debonding of brick. max max 3 x
M
F
d
f
W
W
Table 19 – Out-of-Plane flexural strength and elastic modulus for solid-clay-brick masonry<1945. Solid-clay-brick masonry < 1945
Sample name Year of _{Cons } fx2 Mean Em.fx2(v) Mean Em.fx2(h) Mean
MPa GPa GPa
WIR-H1 B2 1920 1.28 0.83 4.0 3.8 10.6 13.4 B4 0.67 3.3 9.7 B5 0.55 4.0 19.8 Weighted average 0.83 3.8 13.4 Standard deviation 0.39 0.40 5.59 Coefficient of variation 0.47 0.11 0.42
Table 20 – Out-of-Plane flexural strength and elastic modulus for solid-clay-brick masonry>1945. Solid-clay-brick masonry > 1945
Sample name Year of _{Cons } fx2 Mean Em.fx2(v) Mean Em.fx2(h) Mean
MPa GPa GPa
WIL-H2 B1 1952 1.16 1.21 - 7.6 5.6 7.1 B3 1.03 6.0 5.6 B5 1.43 9.1 10.1 BEA-S1 B1 1955 1.38 1.09 6.0 5.4 5.4 4.5 B3 0.84 5.8 4.5 B4 1.06 4.4 3.7 ROE-S2 B2 1955 0.76 1.26 3.1 7.4 3.5 6.4 B5 1.58 9.9 9.7 B6 1.45 9.2 6.0 ROE-S3 B4 1985 0.59 1.14 4.6 4.9 3.4 4.5 B6 1.68 5.1 5.5 KWE-H1 B1 1995 1.38 1.38 4.7 4.7 2.8 2.8 Weighted average 1.22 5.98 5.06 Standard deviation 0.11 2.24 2.32 Coefficient of variation 0.09 0.37 0.46
Table 21 – Out-of-Plane flexural strength and elastic modulus for perforated-clay-brick masonry. Perforated-clay-brick masonry > 1945
Sample name Year of _{Cons } fx2 Mean Em.fx2(v) Mean Em.fx2(h) Mean
MPa GPa GPa
BEA-S2 B4 2001 0.83 0.87 1.9 2.6 2.0 3.1 B5 0.81 2.6 3.8 B6 0.96 3.4 3.4 Weighted average 0.87 2.63 3.07 Standard deviation 0.08 0.75 0.95 Coefficient of variation 0.10 0.29 0.31
Table 22 – Out-of-Plane flexural strength and elastic modulus for other types of masonry. Sample name Year of _{Cons } fx2 Mean Em.fx2(v) Mean Em.fx2(h) Mean
MPa GPa GPa
HOO-H1 - Aerated Concrete B4 2013 0.44 0.47 1.7 1.7 2.3 2.1 B5 0.50 1.7 1.9 JOH-H1- CS elements B3 2008 1.2 1.29 5.7 5.6 7 6.4 B4 1.38 5.4 5.7
Figure 26 – Histogram of out-of-plane flexural strength for all types of clay masonry.
The corresponding graphs for the in-plane bending tests are shown in Appendix C. Again, the specimens displayed brittle behaviour, whereas there were some cases in which the propagation of the cracks was more gradual. An exception were the specimens from ROE-S-1.1 and ROE-S1.2, which were of double-leaf masonry (ROE-S1.1: cross-bond, ROE-S1.2: two parallel walls connected with mortar) and as such still retained a level of residual strength post-peak. The main crack patterns observed are presented in Figure 27 to Figure 29 . Most specimens displayed a typical stepwise crack pattern in the constant moment zone (regardless of whether the joints were properly filled or not), although there were cases of (mostly) straight cracks close to a point of load application or at mid-span. In the case of the double-leaf wallettes, separation between the two leaves was also observed. The effect of the mortar dowels of the BEA-S-2 samples with the perforated clay units is unclear, since the two available results vary greatly. In general, the surface of the units after debonding was clean of mortar, particularly for the calcium silicate samples. The obtained results are presented in Table 23 to Table 28according to masonry unit type and year of construction.
Generally, a scatter in the values of flexural strength was observed. This inconsistency, along with the smaller number of samples that were available for the out-of-plane bending tests (both in terms of particular buildings and of masonry type) does not allow for the extraction of a safe conclusion about the orthotropic bending behaviour of the masonry. Nonetheless, the clay brick wallettes subjected to out-of-plane bending presented almost double the strength as those subjected to in-plane bending, whereas the values for the perforated clay brick samples were almost equal.
Table 23 – In-Plane flexural strength and elastic modulus for solid-clay-brick masonry < 1945. Solid-clay masonry < 1945
Sample name Year of Cons
fx3 Mean Em.fx3(v) Mean Em.fx3(h) Mean
MPa GPa GPa
WIR-H1 B1 1920 1.12 0.75 9.0 7.1 12.2 8.0 B3 0.83 10.4 8.7 B6 0.29 2.0 3.2 ROE-S1.1 B1 1922 0.68 0.51 3.0 4.0 1.5 4.1 B2 0.41 5.2 7.1 B3 0.44 3.7 3.7 ROE-S1.2 B1 1922 0.85 0.57 6.2 3.9 5.7 3.1 B2 0.38 2.0 1.3 B3 0.49 3.5 2.4 Weighted average 0.61 5.00 5.09 Standard deviation 0.12 3.01 3.67 Coefficient of variation 0.20 0.60 0.72
Table 24 – In-Plane flexural strength and elastic modulus for solid-clay-brick masonry > 1945. Solid-clay masonry > 1945
Sample name Year of Cons
fx3 Mean Em.fx3(v) Mean Em.fx3(h) Mean
MPa GPa GPa
WIL-H2 B2 1952 0.35 0.71 0.9 3.4 1.8 3.5 B4 0.38 0.6 0.8 B6 1.4 8.6 7.9 KWE-H1 B2 1995 0.74 0.82 5.9 5.9 4.7 3.4 B3 0.77 7.1 3.6 B4 0.95 4.8 2.0 BEA-S1 B2 1955 0.83 1.06 7.1 9.5 3.7 6.0 B5 1.36 13.2 11.6 B6 0.99 8.3 2.6 ROE-S2 B1 1955 0.57 0.71 1.0 2.6 0.8 2.8 B3 0.67 2.7 4.2 B4 0.88 4.1 3.3 ROE-S3 B1 1985 0.57 0.48 4.1 3.1 8.1 4.6 B3 0.39 2.1 1.0
B5 Problem with recording of force
Weighted average 0.76 4.91 4.04
Standard deviation 0.21 3.60 3.18
Table 25 – In-Plane flexural strength and elastic modulus for perforated-clay-brick masonry. Perforated-clay masonry > 1945
Sample name Year of _{Cons } fx3 Mean Em.fx3(v) Mean Em.fx3(h) Mean
MPa GPa GPa
BEA-S2 B1 2001 1.05 0.81 4.0 3.0 4.5 2.9 B2 0.56 1.9 1.2 B3 Pump Dysfunction Weighted average 0.81 3.0 2.9 Standard deviation 0.35 1.48 2.33 Coefficient of variation 0.44 0.49 0.82
Table 26 – In-Plane flexural strength and elastic modulus for frogged-clay-brick masonry. Frogged-clay masonry > 1945
Sample name Year of _{Cons } fx3 Mean Em.fx3(v) Mean Em.fx3(h) Mean
MPa GPa GPa
HOO-H2 B1
2013
Failure immediately after load application
B4 0.17 0.14 1.9 1.6 2.9 1.75 B6 0.11 1.2 0.6 Weighted average 0.14 1.55 1.75 Standard deviation 0.04 0.49 1.63 Coefficient of variation 0.30 0.32 0.93
Table 27 – In-Plane flexural strength and elastic modulus for calcium-silicate-brick masonry < 1985. Sample name Year of _{Cons } fx3 Mean Em,fx3(v) Mean Em,fx3(h) Mean
MPa GPa GPa
BEA-H1 B3 1958 0.13 0.24 2.4
2.25
1.12.5
B6 0.35 2.1 3.9 LAG-H2 B1 1978 0.46 0.61 1.93.35
1.05.6
B6 0.76 4.8 10.1 SCH-H1 B3 1978 0.41 0.24 3.21.87
2.81.7
B4 0.17 2.0 - B5 0.13 0.4 0.6 Weighted average 0.36 2.5 3.3 Standard deviation 0.23 1.3 3.6 Coefficient of variation 0.63 0.5 1.1Table 28 – In-Plane flexural strength and elastic modulus for other types of masonry. Sample name Year of
Cons
fx3 Mean Em,fx3(v) Mean Em,fx3(h) Mean
MPa GPa GPa
JUL-H1 Concrete blocks B1 1957 0.28 0.31 1.5 1.73 0.6 1.43 B2 0.33 1.8 1.5 B3 0.33 1.9 2.2 HOO-H1 Aerated Concrete B1 2013 0.50 0.58 1.5 1.30 1.8 1.73 B2 0.69 1.5 1.8 B3 0.55 0.9 1.6 JOH-H1 CS elements B1 2008 1.44 0.87 5.4 4.23 6.5 9.30 B2 0.71 4.5 7.4 B5 0.47 2.8 14.0 (a) (b)
Figure 27 – In-Plane Bending – Typical crack patterns: (a) Crack at the point of load application; (b) Straight crack at the middle of the specimen.
Figure 28 – In-Plane Bending – Typical crack patterns: Stepwise debonding in the brick-mortar interface.
(a) (b)
Figure 29 – In-Plane Bending – Double-leaf masonry crack patterns: (a) Front face; (b) Cross section of separation of leaves.
(a) (b)
Figure 30 – Histograms of in-plane flexural strength for: (a) all types of clay masonry; (b) calcium silicate masonry.
8 Bond strength of masonry
The bond wrench strength of bed joints is determined in agreement with EN-1052-5:2005.
8.1 Testing procedure
In total, samples from 14 out of 17 different objects were tested. The tests on 12 of the objects (namely for object codes BEA-S-1/-2, ROE-S-1.1/-1.2/-2/-3, HOO-H-2, WIL-H-1, LAG-H-2, WIR-H-1, JUL-H-1, and KWE-H-1) were performed on specimens saw-cut from the remaining parts of specimens tested in in-plane and out-of-plane bending. For two objects (HOO-H-1 and JOH-H-1) special samples were provided specifically for bond wrench testing. Finally, for objects BEA-H-1, SCH-H-1 and WIL-H-2 no bond wrench tests could be performed, since all samples were broken on delivery and/or during bending tests and subsequent saw-cutting. Any such zero-results were excluded here, although there is an argument to include them in the later interpretation stage of this project.
The specimen is rigidly held by a support frame in accordance with EN 1052-5:2005. A clamp, with a lever attached, is applied to the top unit and the lever is used to create a bending moment in the mortar joint. An analogue scale registers the moment applied. The mortar-brick interface will fail at the location of maximum tensile stress. The apparatus is officially calibrated in the range 20–215 Nm. The tolerance is 4%. Manual readings are accurate to 10 Nm. For some tests, an apparatus calibrated up to 400 Nm was used. Figure 31 shows the test layout.
8.2 Elaboration of data
The bond wrench strength fb,bj is calculated on the assumption that the stress distribution is linear over the
top brick width:
(10)
Where F1 is the failure load, F2is the weight of the bond wrench apparatus, e1 is the distance from the applied
load to the tension face of the specimen, e2 is the distance from the centre of gravity of the clamp to the
tension face of the specimen, F3 is the weight of the masonry unit pulled off the specimen, including the
weight of adherent mortar, b is the mean width of the bed joint, tu is the mean depth of the masonry unit. If
a crushing failure of the masonry unit occurs then the bond strength is not governing and only minimum bond strength, at the point of unit failure, will be known. The type of failure is classified as described in EN-1052-5:2005 (Figure 32).
6
4
3
2
2 3 2 1 2 2 1 1 , u u bj bbt
F
F
F
t
e
F
e
F
f
(a) Type A (b) Type B (c) Type C
(d) Type D (e) Type E (f) Type F
Figure 32 – Classification of failure modes according to EN-1052-5:2005 (1 tension face, 2 compression face).
The results are presented according to masonry unit type in Table 29 to Table 32. Table 29 – Test results for solid clay brick masonry specimens < 1945.
Object Year of _{Cons } Sample _{[MPa] }fb,bj Failure _{Mode } Mean St. Dev. C.o.V.
WIR-H1 1920 1 0.71 Type D 0.60 0.15 0.25 2 0.42 Type D 3 0.70 Type D 4 0.41 Type D 5 0.71 Type D 6 0.62 Type D ROE-S1.1 1922 1 0.34 Type A 0.25 0.11 0.44 2 0.24 Type A 3 0.21 Type B 4 0.39 Type D 5 0.22 Type A 6 0.08 Type A ROE-S1.2 1922 1 0.33 Type C 0.15 0.11 0.74 2 0.09 Type B 3 0.03 Type B 4 0.08 Type C 5 0.21 Type A 6 0.14 Type A
Table 30 – Test results for solid clay brick masonry specimens > 1945. Object Year of _{Cons } Sample fb,bj
[MPa] Failure Mode Mean St. Dev. C.o.V.
WIL-H2 1952 1 0.65 Type D 0.63 0.17 0.28 2 0.47 Type D 3 0.95 Type D 4 0.63 Type D 5 0,48 Type D 6 0,61 Type D BEA-S1 1955 1 0.19 Type A 0.23 0.05 0.19 2 0.20 Type B 3 0.29 Type A 4 0.29 Type B 5 0.22 Type A 6 0.21 Type A ROE-S2 1955 1 0.24 Type C 0.54 0.21 0.40 2 0.40 Type C 3 0.41 Type A 4 0.69 Type B 5 0.76 Type C 6 0.72 Type C ROE-S3 1985 1 0.64 Type A 0.42 0.24 0.58 2 0.52 Type A 3 0.47 Type A 4 0.12 Type A 5 0.12 Type A 6 0.65 Type A KWE-H1 1995 1 0.33 Type A 0.31 0.09 0.29 2 0.47 Type B 3 0.24 Type A 4 0.25 Type A 5 0.35 Type A 6 0.24 Type A
Table 31 – Bond wrench strength for CS masonry samples.
Object Year of _{Cons } Sample fb,bj [MPa] Failure _{Mode } Mean St. Dev. C.o.V.
LAG-H2 1978 1 0.18 Type A 0.18 0.06 0.33 2 0.08 Type A 3 0.22 Type A 4 0.20 Type A 5 0.23 Type A
No other suitable samples were available. SCH-H1 1987 No suitable samples were available. WIL-H1 1952 No suitable samples were available. BEA-H1 1958 No suitable samples were available.
Table 32 - Test results for other specimens. Object Year of
Cons Sample fb,bj [MPa]
Failure
Mode Mean St. Dev. C.o.V.
JUL-H1 Concrete block 1957 1 0.47 Type C 0.23 0.13 0.56 2 0.19 Type C 3 0.26 Type C 4 0.14 Type C 5 0.13 Type C 6 0.18 Type C BEA-S2 Perforated clay brick 2001 1 0.16 Type B 0.15 0.03 0.20 2 0.12 Type A 3 0.16 Type A 4 0.20 Type B 5 0.13 Type A 6 - Crushing HOO-H2 Frogged clay brick 2013 1 0 No bond 0.05 0.046 0.92 2 0.06 Type A 3 0.09 Type A
No other suitable samples were available for testing, due to the poor condition of the original specimens.
HOO-H1 Aerated concrete
block
2013 Crushing of blocks where clamped for small values of M.
JOH-H1 CS
As documented in the above tables, the prevalent modes of failure are type A, i.e. failure at the interface between the upper brick and mortar, and type D, i.e. failure within the mortar joint. Typical failure mechanisms are shown in Figure 33.
Figure 34 shows the failure mechanism for aerated concrete block samples (HOO-H1), which can be attributed to the poor mechanical properties of the units.
Figure 35 presents the histograms of bond strength for all types of clay bricks specimens and calcium silicate specimens.
(a) (b)
Figure 33 - (a) Type A failure (BEA-S-2) and (b) Type D failure (WIR-H-1).
(a) (b)
9 Compressive strength of masonry perpendicular to bed
joints
In this section, the results of cyclic vertical compression tests on masonry are presented, which were performed in TU/e. The values of vertical compressive strength, Young’s modulus (defined as the slope of the most linear part of the stress-strain curve), and compression fracture energy (calculated as the area underneath the stress versus strain (based on the LVDTs displacement) times average of LVDTs length curve) are reported.
Table 33 - Table 37 list the main experimental results of the calcium silicate, clay, concrete, and aerated concrete wallettes.
Table 33 – Results of vertical compression tests on calcium silicate masonry < 1985. Sample
name fm,v MPa Mean Echord,v MPa Mean Gf-c,v N/mm Mean
BEA-H1 6.02 5.72 5491 3984 10.79 12.54 5.42 2476 14.28 WIL-H1 9.97 9.55 5882 6276 21.57 22.72 9.12 6669 23.87 LAG-H1 13.45 14.15 9909 9156 36.27 35.22 15.78 9163 34.17 13.22 8395 - SCH-H1 13.69 13.63 11481 9293 15.12 15.55 12.97 9875 23.18 13.27 8268 11.73 14.60 8348 12.16 13.63 8491 - Weighted average 10.76 7177 21.51 Standard deviation 3.94 2543 10.09 Coefficient of variation 0.37 0.35 0.47
Table 34 – Results of vertical compression tests on clay masonry < 1945. Sample
name fm,v [MPa] Mean Echord,v [MPa] Mean Gf-c,v [N/mm] Mean WIR-H1 14.54 14.40 12872 13675 - - 14.94 14477 - 13.72 - - MID-H1 12.02 12.01 5471 4613 47.19 40.91 13.17 4436 - 10.85 3933 34.63 15.84 12.14 4388 3864 24.01 24.01 10.95 3339 - 9.61 - - ROE-S1 11.77 11.62 9560 10054 16.40 19.42 9.25 10548 18.50 12.80 - 23.38 10.59 - - 13.70 - - MOL-H1 4.35 4.00 3843 3568 - 9.50 4.50 4048 9.29 3.09 2813 9.72 3.85 3.92 2445 1690 9.01 6.85
4.79 1355 6.02 3.11 1269 5.53 Weighted average 9.68 6244 20.14 Standard deviation 4.54 4603 13.57 Coefficient of variation 0.47 0.74 0.67
Table 35 - Results of vertical compression tests on clay masonry > 1945. Sample
name fm,v [MPa] Mean Echord,v [MPa] Mean Gf-c,v [N/mm] Mean BEA-S1 13.99 14.05 8804 6779 15.18 17.03 16.54 6301 12.85 16.50 8662 11.06 11.97 2213 29.03 11.27 7916 - KWE-H1 11.48 10.56 7287 5930 - 27.11 11.18 5631 24.35 10.17 6980 19.62 9.39 3821 37.37 WIL-H2 22.96 20.51 14696 12348 14.04 18.86 20.15 9666 29.47 18.43 12681 13.06 ROE-S3 9.38 9.10 7151 4332 - 29.67 9.77 3876 35.36 8.29 3716 22.33 8.96 2584 31.31 28.60 28.01 9851 8419 - 33.63 27.41 6986 33.63 BEA-S2 19.44 20.74 10918 8688 25.85 27.19 20.93 9998 - 18.86 8098 - 21.41 8121 27.46 22.18 6883 23.82 18.17 6718 25.92 26.26 11327 32.92 18.66 7444 - ROE-S2 12.91 15.43 15248 13262 13.28 16.27 18.12 15366 9.72 12.27 7876 13.74 16.09 12218 28.34 17.78 15604 - HOO-H2 8.40 7.95 2575 2575 6.40 8.87 8.07 1199 11.96 7.35 1806 - 8.05 3423 5.29 7.89 3871 11.83 Weighted average 15.79 7792 22.33 Standard deviation 6.89 3695 8.33 Coefficient of variation 0.44 0.47 0.37